1 AN ABSTRACT OF THE THESIS OF Abdul la Ali Al-Joaib for the degree of Doctor of Philosophy in Civil Engineering presented on May Title: Evaluation of Water Damage on Asphalt Concrete Mixtures Using The Environmental Conditioning System Abstract Approved: Redacted for Privacy Dr. Ronald L. Terrel Asphalt concrete pavement is subjected to several damaging actions from traffic loads, water (from precipitation and/or groundwater sources), and temperature. The durability of the asphalt-aggregate mixture, its ability to withstand these damaging actions for long periods, is a very important engineering property. While the durability of the asphalt-aggregates mixture depends on several factors such as the mixture's properties, construction methods, traffic loads and environmental conditions, they have to be evaluated to predict their field performance. Based on mixture evaluations, the mixtures that fail the test would have to be modified by additives or by changing the materials. The first objective of this thesis was to evaluate asphalt-aggregate mixtures for water damage using the Environmental Conditioning System (ECS), and rank the asphalt and aggregate types based on water sensitivity. The second objective was to relate the ECS ranking of the asphalt and aggregate types to Oregon State University (OSU) and University of Nottingham, UK (SWK/UN) wheel tracking test results, and to Net Adsorption Test (NAT) results. The third objective was to evaluate open-graded mixtures and rubber modified mixtures for water sensitivity using the ECS. The ECS test results indicate that performance ranking of mixtures by asphalt type or aggregate type alone cannot be made for the ECS test results due to the significant interaction between asphalt and aggregate. Water sensitivity in the ECS is
2 significant for combinations of asphalt and aggregate. The ECS test results have shown that ECS performance ranking after one cycle is not statistically significant and does not correlate with ranking after three cycles. The results show that the ECS test program has similar aggregate rankings to those of the NAT and SWK/UN test program, while good agreement exists between SWK/UN wheel tracking results and the NAT test program results. However, poor agreement exists between the OSU wheel tracking results and those of the other two tests. Poor or very little agreement exists among the wheel tracking test results, ECS, and NAT test results in terms of asphalt type rankings. When considering the comparisons of materials ranking by different test procedures, one must keep in mind that the mechanisms leading to varying "performance" are not the same. The testing reported herein was aimed at measuring water sensitivity, but all the tests do not do so directly. The NAT procedure addresses only the potential for stripping (adhesion) and is not capable of evaluating cohesion loss. The other tests (ECS, OSU and SWK/UN wheel tracking) included all the mechanisms simultaneously, and these provided a gross effect without clearly separating the cause of failure in each case. Open-graded mixtures used by Oregon Department of Transportation (ODOT) performed well in the ECS in terms of water sensitivity. In the ECS evaluation, six mixtures passed the criteria of 75 % established for Indirect Retained Strength (IRS) test by ODOT, and one mixture was marginal. However, only one mixture passed the IRS evaluation, and another mixture was marginal. This confirms that the IRS test is a very severe test and is not suitable for water sensitivity evaluation of open-graded mixtures. Finally, the IRS test evaluation would suggest that these mixtures would fail prematurely after construction, but all of these mixtures have been used in projects which have been in service for more than three years with no visible signs of distress, or failures.
3 EVALUATION OF WATER DAMAGE ON ASPHALT CONCRETE MIXTURES USING THE ENVIRONMENTAL CONDITIONING SYSTEM by Abdulla Ali Al-Joaib A THESIS submitted to Oregon State University in partial fulfillment of the requirements for the degree of Doctor of Philosophy Completed May 28, 1993 Commencement June, 1994
4 Copyright 1993 by Abdul la Ali Al-Joaib May 28, 1993 All Rights Reserved
5 APPROVED: Redacted for Privacy Ronald L. Terrel, Ph.D. Professor of Civil Engineering in charge of major Redacted for Privacy Wayne C. H er, Ph.D. Head Department of Civil Engineering Redacted for Privacy Thomas J. Maresh, Ph.D. Dean of Graduate School Date thesis is presented Typed by May 28, 1993 Abdulla Ali Al-Joaib
6 ACKNOWLEDGMENT This research was made possible through a contract with the Strategic Highway Research Program (SHRP), project A-003A "Performance Related Testing and Measuring of Asphalt-Aggregate Interactions and Mixtures", the University of California at Berkeley, and Oregon State University. SHRP is a unit of the National Research Council that was authorized by section 128 of the Surface Transportation and Uniform Relocation Assistance Act of I wish to express my gratitude to my father and mother, to my wife, and my son for their patience, devotion, and encouragement during the years of my study. I would like to thank my major professor, Dr. Ronald Terrel for his support, invaluable consultation, and encouragement during the course of my study. In particular, the knowledge, experience, and friendship is greatly appreciated. I would also like to thank Dr. Gary Hicks for his invaluable direction, and guidance during my project, and my graduate committee members: Dr. John Peterson, Dr. Benno P. Warkentin, and Dr. Harold D. Pritchett, for their time and assistance. Finally, thanks go to all of my friends in the Civil Engineering laboratory and water sensitivity group: Todd Scholz, Dr. Saleh Al-Swailmi, Andy Brickman, Wendy Allen, and Larry Ilg.
7 TABLE OF CONTENTS PAGE 1.0 INTRODUCTION PROBLEM DEFINITION 1.2 OBJECTIVES LITERATURE REVIEW DEFINITION OF WATER DAMAGE EXISTING METHODS TO EVALUATE WATER DAMAGE SELECTION OF ECS EXPERIMENT DESIGN VARIABLES CONSIDERED MATERIALS Aggregates and Their Properties Asphalts and Their Properties SPECIMEN PREPARATION TESTING METHODS OSU ECS Test OSU Wheel Tracking Test SWK/UN Wheel Tracking Test TEST RESULTS ECS TEST PROGRAM Discussion of ECS Test Program Results OSU WHEEL TRACKING PROGRAM SWK/UN WHEEL TRACKING PROGRAM 59
8 TABLE OF CONTENTS (Continued) PAGE 4.4 UNR NET ADSORPTION TEST PROGRAM ANALYSIS OF RESULTS STATISTICAL ANALYSIS ECS Test Results OSU Wheel Tracking Test Results SWK/UN Wheel Tracking Test Results UNR Net Adsorption Test Results PERFORMANCE RANKING Aggregates Asphalts Mixtures PERFORMANCE RANKING COMPARISONS EXTENDED TEST PROGRAM EVALUATION OF OPEN GRADED MIXTURES Oregon Open-graded Mixtures Washington Open-graded Mixtures AUSTRALIAN MODIFIED MIXTURES STUDY CONDITIONING CYCLE DURATION STUDY CONCLUSIONS AND RECOMMENDATIONS CONCLUSIONS RECOMMENDATIONS FOR IMPLEMENTATION RECOMMENDATIONS FOR FUTURE RESEARCH 120 BIBLIOGRAPHY 122
9 TABLE OF CONTENTS (Continued) PAGE APPENDICES APPENDIX A APPENDIX B APPENDIX C APPENDIX D APPENDIX E APPENDIX F APPENDIX G APPENDIX H APPENDIX I SAMPLE PREPARATION 125 TEST PROCEDURES 141 SHRP MIXTURES TEST DATA 180 EC S FIGURES 197 STATISTICAL ANALYSIS 207 OREGON DEPARTMENT OF TRANSPORTATION 228 PROJECT WASHINGTON DEPARTMENT OF 251 TRANSPORTATION PROJECT SUMMARY DATA OF AUSTRALIAN PROJECT 258 SUMMARY DATA OF CYCLE DURATION STUDY 260
10 LIST OF FIGURES PAGE Figure 2.1 Figure 2.2 Figure 3.1 Figure 3.2 Figure 3.3 Figure 3.4 Figure 3.5 Figure 3.6 Figure 3.7 Figure 3.8 Figure 4.1 Figure 4.2 Figure 4.3 Figure 4.4 Figure 4.5 Figure 4.6 Figure 4.7 Figure 4.8 Figure 4.9 Figure 4.10 Figure 4.11 Figure 5.1 Figure 5.2 Figure 5.3 Water Damage Triangle (Graf, 1986) Schematic of Environmental Conditioning System Schematic of the Specimen Preparation Process Asphalt-aggregate Mixer Used at OSU The Compacted Slab Layout of Specimens Cut From the Slab The OSU Wheel Tracker Schematic of the OSU Wheel Tracker Deformation Measurement Positions in the OSU wheel Tracker Schematic of the SWK/UN Wheel Tracker ECS Test Results for the RC Aggregate ECS Test Results for the RD Aggregate ECS Test Results for the RH Aggregate ECS Test Results for the RJ Aggregate The Effect of ECS Conditioning on Water Permeability of RC Mixes The Effect of ECS Conditioning on Axial Deformation of RD Mixes OSU Wheel Tracking Test Results for the RC Aggregate OSU Wheel Tracking Test Results for the RD Aggregate OSU Wheel Tracking Test Results for the RH Aggregate OSU Wheel Tracking Test Results for the RJ Aggregate Net Adsorption Test Results ECS Performance Ranking of Mixtures Based on One and Three Cycles ECS Performance Ranking of Mixtures Based on Three and Four Cycles Comparisons between Performance Rankings of Mixtures by Stripping and ECS-MR
11 LIST OF FIGURES (Continued) PAGE Figure 5.4 Comparisons of Performance Rankings by ECS and NAT 103 Test Figure 5.5 Comparisons of Performance Rankings by Stripping and 103 NAT Tests Figure 6.1 Plot of Diametral and Air Voids Results For Mix A- ODOT 106 Figure 6.2 Summary of Open-graded Mixtures Results ODOT 106 Figure 6.3 Effect of ECS Test on Open-graded Mixtures - WSDOT 109 Figure 6.4 ECS Evaluation of Australian Modified Mixtures Figure 6.5 Effect of Cycle Duration on ECS Evaluation of Mixture B 112 Figure 6.6 Effect of Cycle Duration on ECS Evaluation of Mixture C 112 Figure 7.1 ECS Criteria Concept Water Sensitivity Evaluation 118 Figure 7.2 ECS Criteria Concept- Design Based on Air Voids
12 LIST OF TABLES PA E Table 2.1 Factors Influencing Water Damage (Hicks, 1991) 7 Table 2.2 Factors Influencing Water Sensitivity of Asphalt-Aggregate Mixtures ( Terrel and Shute, 1989) 11 Table 2.3 ECS Test Procedure (Terrel and Al-Swailmi, 1992) 14 Table 3.1 Experiment Design for ECS Evaluation of 32 SHRP Mixtures Water Sensitivity 17 Table 3.2 Experiment Design of ECS Evaluation of 32 SHRP Mixtures Water Sensitivity Table 3.3 Job-Mix Formula Used for SHRP Mixtures -Water Sensitivity Table 3.4 Aggregate Characteristics (Scholz et al., 1993) Table 3.5 Asphalt Characteristics (Scholz et al., 1993) Table 3.6 Table 3.7 Table 3.8 Table 4.1 Table 4.2 Table 4.3 Table 4.4 Table 4.5 Table 4.6 Table 4.7 Table 4.8 Summary of Specimen Preparation Procedure for ECS Evaluation of SHRP Mixtures - Water Sensitivity Summary of OSU Wheel Tracking Test Procedure Summary of SWK/UN Wheel Tracking Procedure Summary of ECS Tests Data for RC Mixes Summary of ECS Tests Data for RD Mixes Summary of ECS Tests Data for RH Mixes Summary of ECS Tests Data for RJ Mixes Summary of Mixtures Tested in OSU Wheel Tracking Program Rut Depths for the OSU Wheel Tracking Program Summary Results of SWK/UN Wheel Tracker Test Program Net Adsorption Test Results
13 LIST OF TABLES (Continued) PAGE Table 5.1 Table 5.2 Variables Considered in the Statistical Analyses of the ECS Test Results An Overview of the ECS Statistical Analyses Table 5.3 GLM Analysis of the ECS Results for Asphalt and Aggregate 76 Table 5.4 Type GLM Analysis of the ECS Results 78 Table 5.5 GLM Analysis of the ECS Results and Materials' Properties 81 Table 5.6 GLM Analysis of the OSU Wheel Tracking Test Results 81 Table 5.7 Extended GLM Analysis of the OSU Wheel Tracking Test 83 Table 5.8 Results Bayesian Survival Analysis of the SWK/UN Test Results 85 Table 5.9 GLM Analysis of the NAT Results for Asphalt and Aggregate 87 Type Table 5.10 Performance Ranking of Aggregates Based on ECS Test 89 Table 5.11 Performance Ranking of Aggregates (OSU Wheel Tracking Program) Table 5.12 Performance Ranking of Aggregates (SWK/UN Wheel Tracking Program) Table 5.13 Performance Ranking of Aggregates (NAT/UNR Test Program) Table 5.14 Performance Ranking of Asphalt Based on ECS Test Table 5.15 Performance Ranking of Asphalts (OSU Wheel Tracking Program) Table 5.16 Performance Ranking of Asphalts (SWK/UN Wheel Tracking Program)
14 LIST OF TABLES (Continued) PAGE Table 5.17 Performance Ranking of Asphalts (NATIUNR Test Program) 94 Table 5.18 Ranking of 32 Mixes After Each ECS Cycle 95 Table 5.19 Summary of Aggregate Rankings 101 Table 5.20 Summary of Asphalt Rankings 101
15 LIST OF APPENDICES FIGURES PAGE Figure Al Figure A2 Figure A3 Figure A4 Figure B1 Figure B2 Figure B3 Figure B4 Figure B5 Figure B6 Figure B7 Figure B8 Figure B9 Rolling Wheel Compactor Schematic of Mold for Slab Bitumen Test Data Chart Preheating the Mold Environmental Conditioning System (Front View) Load Frame with Specimen Control Panel Groove Pattern for End Platens Perforated Teflon Disks Conditioning Cycles for Warm and Cold Climates Stripping Rate Standards Binder Migration Standards Illustration of Specimen Deformation Resulting from Application of Load Cycles Figure D1 Figure D2 Figure D3 Figure D4 Figure D5 Figure D6 Figure D7 Figure D8 Figure D9 The Effect Of ECS Conditioning on Asphalt AAA-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAB-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAC-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAD-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAF-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAG-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAK-1 Mixtures The Effect Of ECS Conditioning on Asphalt AAM-1 Mixtures The Effect Of ECS on Water Permeability of Aggregate RC Mixtures Figure D10 The Effect Of ECS on Water Permeability of Aggregate RD 202 Mixtures Figure Dll The Effect Of ECS on Water Permeability of Aggregate RH 203 Mixtures Figure D12 The Effect Of ECS on Water Permeability of Aggregate RJ 203 Mixtures Figure D13 Effect of Latex Membrane on Air Permeability 204
16 LIST OF APPENDICES FIGURES (Continued) PAGE Figure D14 Axial Deformation For Aggregate RC Mixtures Figure D15 Axial Deformation For Aggregate RD Mixtures Figure D16 Axial Deformation For Aggregate RH Mixtures Figure D17 Axial Deformation For Aggregate RJ Mixtures Figure Fl Plot of Diametral MR and Air Voids Results for Mixture A Figure F2 Summary of Open-graded Mixtures Results Figure F3 Comparisons Between ECS-MR, Stripping, and IRS Results Figure F4 Effect of Additive on Mixture Performance in ECS Figure F5 Comparisons of ECS and IRS Performance Ranking Figure G1 Comparisons Between ECS and IRS Results Figure G2 Effect of Additive on Mixture Performance in ECS Figure G3 Relationship Between Air Voids and Permeability to ECS Results
17 LIST OF APPENDICES TABLES I:AWE Table B1 Table Cl Table C2 Table C3 Table Fl Table F2 Table F3 Table G1 Table H1 Table Il Minimum Test System Requirements Summary Data of 32 SHRP Mixtures - ECS Summary Data of 32 SHRP Mixtures - SWK Summary Data of 32 SHRP Mixtures OSU Wheel Tracker Summary of ODOT Projects Summary of ODOT Open-graded Mixtures GLM Analysis of the Open-graded Mixtures Study Summary Data of WSDOT Open-graded Mixtures Summary of ECS Data for Australian Modified Mixtures Summary of ECS Data for Cycle Duration Study
18 EVALUATION OF WATER DAMAGE ON ASPHALT CONCRETE MIXTURES USING THE ENVIRONMENTAL CONDITIONING SYSTEM 1.0 INTRODUCTION 1.1 PROBLEM DEFINITION Asphalt concrete pavement is subjected to several damaging actions from traffic loads, water (from precipitation and/or groundwater sources), and temperature. The durability of the pavement, the ability of the pavement to withstand these damaging actions for long periods, is a very important engineering property. While the durability of the asphalt concrete pavement depends on several factors such as mixture properties, construction methods, traffic loads and environmental conditions, asphalt concrete mixtures have to be evaluated to predict their field performance. Based on mixture evaluations, those mixtures that fail the test would have to be modified by additives or by changing the materials. The main goal is to design and construct a pavement that, in the long term, can resist all damaging actions, whether they are from the environment (water, and temperature), or traffic loads. Since the 1930's, researchers have been trying to develop a test that would determine the susceptibly of water damage on asphalt concrete mixtures (Terrel and Shute, 1989). Several tests have been developed that try to simulate water damage on asphalt mixtures, and then assess the damage by evaluating mixture strength loss. However, most of the different water sensitivity tests have been unsuccessful in predicting the premature failures in asphalt concrete pavements due to water damage. The problem with some of these tests is that they do not relate to field conditions. Typically, water sensitivity tests are two-step procedures: mixture conditioning, and mixture evaluation. In the first step, the mixture is subjected to a
19 2 conditioning process that attempts to simulate the damage caused by environmental conditions in the field. Next, the mixture is evaluated for any deterioration in strength caused by water damage by evaluating the mixture strength before and after conditioning. Some of the evaluation methods used are strength or modulus testing, then the ratio of before and after conditioning is determined. If the ratio is less than a specified value, then the mixture has failed the water sensitivity test. Visual evaluation of stripping is also used where the percentage of retained asphalt coating on the aggregate is determined. The laboratory conditioning process by which the water damage is induced does not relate to what actually occurs in the field. Also, some of these tests do not relate to water damage failure mechanisms that would develop. Damage caused by water is a combination of several failure mechanisms: adhesion loss, cohesion loss, and aggregate degradation (Hicks, 1991). One of Strategic Highway Research Program (SHRP) goals was to develop a performance based test that could predict the influence of water damage on asphalt-aggregate mixtures. The Environmental Conditioning System was developed at OSU as part of SHRP's efforts to develop a test that could rank asphalt aggregate mixtures with respect to susceptibility to water damage (Terrel, and Al-Swailmi, 1991). Although the ECS test cannot separate the different failure mechanisms, the ECS test has a more realistic conditioning procedure and can evaluate the physical behavior of asphalt concrete mixtures when water is present. 1.2 OBJECTIVES Part of this research effort was conducted as part of SHRP project A-003A "Performance Related Testing and Measuring of Asphalt-aggregate Interactions and Mixtures." The primary objective of the A-003A project was to validate the relationships between asphalt binder properties and asphalt concrete mixtures performance. The secondary objective was to develop accelerated mixture performance
20 test procedures to be included in the SHRP mix design specifications. The primary purpose of this portion of the SHRP A-003A project was to validate the ECS and preliminary ranking of asphalts developed by other SHRP projects (Schloz et al., 1993). The objectives of this research were to: 1) Evaluate thirty-two SHRP asphalt-aggregate mixtures for water damage using the ECS, and rank the asphalt and aggregate types based on water sensitivity tests, 2) Relate the ECS ranking of the asphalt and aggregate types to OSU and SWK/UN wheel tracking test results, and to NAT results, 3) Evaluate open-graded asphalt mixtures from the Washington Department of Transportation (WSDOT) and the Oregon Department of Transportation (ODOT) for water sensitivity using the ECS, 4) Evaluate modified asphalt-aggregate mixtures from Australia for water sensitivity using the ECS, and 5) Evaluate the ECS conditioning cycle duration. 3
21 4 2.0 LITERATURE REVIEW The literature review of the water sensitivity problem was divided into three parts. First, water sensitivity failure mechanisms and factors that might influence water damage were reviewed. Second, a review of existing methods to evaluate water damage potential was performed. Finally, factors that lead to the selection of the Environmental Conditioning System as a suitable test to evaluate the susceptibility of mixtures to water damage were completed. 2.1 DEFINITION OF WATER DAMAGE Water damage is a major phenomenon that causes distress and failures in asphalt concrete pavement due to the presence of water, temperature, and traffic loading. The best analogy that illustrates water damage theory and the factors influencing water damage potential is shown in Figure 2.1, "Water Damage Triangle" (Graf, 1986). First, the material's sensitivity in the presence of water and any of the distress can affect the water damage. In some regions of the USA where the climate is mild and there are good quality aggregates and asphalt cement, the major contribution to pavement deterioration may be due to traffic loading. However, in other regions of the country where there are poor aggregates and/or asphalt cement, coupled with severe weather and traffic loading, premature failure may occur. The water damage triangle analogy shows the complexity involved in understanding this problem. The understanding of the water damage phenomenon is tied very much to our understanding of the failure mechanisms that occur, causing premature failures in the pavement. There are several factors that can affect water damage potential and the performance of asphalt concrete mixture in the presence of water. These factors can be grouped into three categories (Hicks, 1991):
22 5 Modifiers Asphalt Type 1 Aggregate Type Materials Sensitivity Mixture Type /Traffic Loading Water Stresses 4-- Temperature 1\ Environment Figure 2.1 Water Damage Triangle (Graf, 1986)
23 6 1) Mixture characteristics, which include aggregate, asphalt, mixture type, 2) Weather during construction, and 3) Environmental conditions after construction. Table 2.1 summarizes the factors that might influence water damage potential in asphalt concrete mixtures and their desirable characteristics. Although aggregates constitute about 90 to 95 percent of the asphalt concrete mixture weight, the aggregate effect on the mixture's performance is not proportionally dependent on the relative weight of aggregate to asphalt. The surface texture of the' aggregate affects the coatability of the aggregate by asphalt, and the mechanical retention of the asphalt coating as well. Aggregates that have rough surfaces when coated with asphalt require more energy to be displaced by water, thus improving the water resistance. Also, the surface coating affects the adhesion, and porosity promotes adhesion due to mechanical lock. Mineralogical and chemical composition affect the aggregate's surface chemical reactivity. Aggregates possessing certain chemicals tend to behave differently when moisture is present, and the potential of asphalt being displaced by water is dependent on the aggregate's chemical composition. Aggregate types which are classified as "acidic" aggregates have been shown to have more affinity for water than "basic" aggregates (Rice, 1958). In other words, acidic aggregates tend to strip more, thus causing premature failure in the asphalt concrete pavement. However, other researchers have found that the notion that "acidic" rocks have a higher potential for stripping than "basic" aggregate is inaccurate (Terrel and Shute, 1989). Aggregate surface zeta potential in water and/or ph of water penetrating the aggregate could be used as a measure of stripping potential, where higher zeta potential and/or ph value would lead to higher stripping potential (Terrel and Shute, 1989).
24 7 Table 2.1 Factors Influencing Water Damage (Hicks, 1991) Factor Desirable Characteristics 1) Aggregate Type Surface Texture Rough Porosity Depends on pore size Mineralogy Basic aggregates are more resistant Dust Coatings Clean Surface Moisture Dry Surface Chemical Composition Able to share electrons or form hydrogen bond Mineral Filler Increases viscosity of asphalt 2) Asphalt Cement Viscosity Chemistry Film Thickness 3) Type of Mixture Voids Gradation Asphalt Content 4) Weather Conditions Temperature Rainfall During Construction Rainfall after Construction Freeze-Thaw High Nitrogen and phenols Thick Very low or very high Very dense or very open High Warm None Minimal Minimal 5) Traffic Loading Low Traffic
25 Knowledge or theories to link asphalt properties to water damage have not been developed. There is evidence that viscous asphalts are not affected as much by moisture as less viscous asphalts. The asphalt viscosity has been reported as an important asphalt property in determining the water damage potential (Majidzadeh and Brovold, 1968). Asphalt types with higher viscosity values can resist the displacement by water more than asphalts with lower viscosity, because higher viscosity asphalt coats the aggregate surface with a thicker film which protects the aggregate from the action of water. Adhesion stripping studies on different asphalt types have not shown any correlation between the asphalt properties and stripping-adhesion failure mechanisms. Premature failure of asphalt concrete pavement due to water damage is caused by a combination of several failure mechanisms (Hicks, 1991): 8 1) Adhesion loss, 2) Cohesion loss, and 3) Aggregate degradation. Adhesion loss occurs when the asphalt film is partially separated from the aggregate by water; this is the case when an aggregate has a greater affinity for water than for asphalt. There are a number of theories that have been developed to explain adhesion loss, but no single theory seems to explain adhesion. All of the adhesion theories have been developed around material properties that would relate to the asphalt-aggregate interface (see Table 2.1). In a compacted mixture, cohesion can be described as being the over all integrity of the material when subjected to load or stress. Cohesive strength can be measured by the resilient modulus test, or tensile strength test. The cohesion is influenced by the viscosity of the asphalt filler system. Cohesion loss occurs when asphalt film is separated by water, i.e., when rupture in the asphalt film occurs.
26 9 The third failure mechanism is aggregate degradation, and this is aggregate failure in the asphalt concrete mixture due to water saturation, environmental factors, and loading stresses. This failure mechanism occurs with poor aggregates in terms of strength and not necessarily in terms of water sensitivity. Aggregates that have high water absorption, coupled with lower strength, tend to absorb water and disintegrate, thus leading to mixture failure. The different failure mechanisms cannot be separated, because in one way or another these mechanisms act together (Terrel, 1991). The evaluation methods such as the resilient modulus test, tend to measure gross effects of these failure mechanisms, and cannot be separated. 2.2 EXISTING METHODS TO EVALUATE WATER DAMAGE Since the 1930's numerous studies have been conducted in the water damage area, and several test methods have been developed to test asphalt concrete mixtures for water damage potential (Terre! and Shute, 1989). Table 2.1 shows factors that should be considered when developing a water sensitivity test. The water sensitivity tests are divided into two categories: 1) Tests which coat a "standard" aggregate with an asphalt cement with or without an additive. The loose uncompacted mixture is immersed in water, either at 25 C or at boiling temperature. The loose mixture is evaluated visually, by assessing the separation or stripping of asphalt from the aggregate. 2) Tests which use laboratory compacted specimens, or cores from the field. The specimens are conditioned in a certain procedure to simulate the field conditions. The specimens are evaluated by taking the ratio of conditioned and unconditioned test results, e.g. diametral resilient modulus test, diametral tensile strength, etc.. These water sensitivity tests rate the performance of the asphalt concrete mixture by using such terms as "reasonable," "good," and "fair." The problem with all
27 of these tests is that the evaluation method and rating seldom relate to field performance. Variability in the test parameters can affect the evaluation and decrease the precision of the results. The mixture evaluated in the lab might have a "good," or pass rating, but still fail prematurely in the field. Different tests, like AASHTO T 283, Tunnicliff and Root, Boiling, Freeze-Thaw Pedestal, and Immersion-Compression tests have been used to predict mixture field performance (Hicks, 1991). Each test has its advantages and disadvantages. The major problem with existing tests is a lack of good correlation with field performance with respect to water induced damage (Hicks, 1991). Also, some of these tests do not relate to water damage failure mechanisms that would develop. The most important disadvantage of water sensitivity tests is that the conditioning is too severe (torture test), and laboratory conditioning does not relate to conditioning in the field. Moreover, the evaluation methods of some of these tests are very subjective and do not relate to any engineering evaluation method SELECTION OF ECS For the research presented here, the Environmental Conditioning System (ECS) was selected as the primary test for water sensitivity evaluation of asphalt concrete mixtures. The ECS was developed as part of the SHRP project. The goal was to relate asphalt mixture properties to performance of mixtures. The ECS was devised, and assembled for water sensitivity testing and evaluation. The ECS test procedure was developed as part of an extensive testing program (Terrel, and Al-Swailmi, 1992). In the development phase of the ECS, many variables were considered and tested. For example, some of the variables were permeability, conditioning level, cycle duration, conditioning time, rate of wetting, aging, loading, air voids, etc. (see Table 2.2).